**Ab initiostudies of the**

**phase transitions inK2SeO4**

**The Harvard community has made this**

**article openly available. Please share how**

**this access benefits you. Your story matters**

### Citation

### Lu, H. M., and J. R. Hardy. 1990. “Ab Initiostudies of the Phase

### Transitions inK2SeO4.” Physical Review B 42 (13) (November 1):

### 8339–8350. doi:10.1103/physrevb.42.8339.

### Published Version

### doi:10.1103/PhysRevB.42.8339

### Citable link

### http://nrs.harvard.edu/urn-3:HUL.InstRepos:32417867

### Terms of Use

### This article was downloaded from Harvard University’s DASH

### repository, and is made available under the terms and conditions

### applicable to Other Posted Material, as set forth at http://

PHYSICAL REVIEW B VOLUME 42, NUMBER 13 1 NOVEMBER 1990

**Ab **

**Ab**

**initio **

**initio**

**studies of the phase transitions in K2SeO4 **

H . M. Lu and J. R. Hardy
* Department of Physics and Center for Electro-Optics, University of Nebraska-Lincoln, Lincoln, Nebraska 68588-0111 *
(Received 18 June 1990)

An * ab initio model is developed for the potentials in ionic molecular solids in which the electron *
covalency within the molecular ions substantially affects the interionic interactions. By treating the
intermolecular and intramolecular interactions on the basis of the true electron charge densities of
the molecular ions, this new model leads to an accurate parameter-free description of the potential-
energy surfaces for such crystals. We performed first-principles static structural relaxation, super-
cell molecular-dynamics simulation, and lattice-dynamics studies for the room-temperature
paraelectric phase and the lower-temperature ferroelectric superstructure of K,Se04 and predicted
with good accuracy the transition from the former to the latter. Given the excellent agreement be-
tween theory and experiment, we then explored the delicately balanced potential-energy surfaces for
K2Se04 and found that they contain a double-well type of structure which is the essential origin of
the incommensurate and the subsequent commensurate transitions in K2Se04.

I. INTRODUCTION

As one of the earliest insulators to exhibit an incom-
mensurate phase, potassium selenate (K2Se04) has at-
tracted extensive experimental and theoretical efforts.'
In the room-temperature (paraelectric) phase the crystal
is orthorhombic with space-group Pnam *(0:; * At
129.5 K it undergoes a displacive type of structural phase
transition into an incommensurate phase, as is evidenced
by the presence of satellite peaks in x-ray3 and neutron-
scattering4 studies. The neutron experiments show that
this structural instability is driven by a soft phonon with
a wave vector q =

*f *

[ ( 1 **-6)a*],**where a* is the first reciprocal-lattice vector along the [I001 direction. As the crystal is cooled further, 6 decreases and vanishes abrupt- ly at 93 K , when the system locks into a commensurate superstructure whose a axis is triple the size of that of the room-temperature phase. The structure of this new phase is also orthorhombic with space group Pna2,

*(c;,) *

and the crystal acquires a spontaneous polarization along
the c axis.
The first theoretical work on a microscopic basis for K2Se04 was by Haque and ~ a r d ~ . ~ With the short- range forces in a rigid-ion model determined by using the equilibrium constants and the observed Brillouin-zone- center frequencies, they performed lattice-dynamics stud- ies on the basis of a quasiharmonic approximation and found that the lowest-lying 8, branch indeed has a minimum near q = a * /3, in agreement with the neutron- scattering r e s u l k 4 A n important finding of this work is the fact that the origin of the instability responsible for the incommensurate and the ferroelectric phase transi- tions is the near cancellation between large Coulomb and short-range forces. This suggests that a reliable under- standing of the transition mechanism has to be based on an accurate description of both components of the in- terionic interactions, and thus of their difference~.

In this paper we describe first-principle simulations of

K2Se04 using ab initio interionic potentials. Such simula- tions have proved very successful in explaining melting,6 superionicity,' zone-boundary instabilities in halide perovskites,8~9 as well as incommensurate phase transi- t i o n ~ . ' ' - ' ~ By using the Gordon-Kim electron-gas mod- ell3 to compute the short-range potentials directly from a b initio electron charge-density distributions of the indi- vidual ions, this approach provides, within the rigid-ion and pairwise interaction approximation, realistic potential-energy surfaces for crystals and therefore allows clear and reliable discrimination between delicately bal- anced structural instabilities.

The most basic assumption underlying the original Gordon-Kim model is that, for closed-shell ions, the total electron charge-density distribution of an ion pair is a su- perposition of the charge densities of the individual ions. While such an assumption seems valid for strictly ionic crystals, it becomes inapplicable to crystals that contain molecular ions, i.e., ionic molecular crystals, to which class K,Se04 belongs. More specifically, this assumption could be invalid when the ion pair in question consists of atoms that are parts of the same molecular ion, e.g., an Se-0 pair within the selenate ion ~e0:-. This is so be- cause there could be marked electron covalency within the molecular ions, as is certainly the case for the selen- ate. O n one hand, this covalency renders the total elec- tron charge distribution inexpressible by a simple super- position of the electron charge distributions of the con- stituent atoms and therefore prohibits the use of Gordon-Kim potentials for the intramolecular interac- tions. O n the other hand, the covalency alters the elec- tronic populations on the individual atoms substantially from the closed-shell configurations so that interactions external t o the molecular ions are also affected. More- over, the electron covalency introduces many-body and/or noncentral interactions, which fall outside of the scope of the usual pairwise-central-force scheme.

In fact, such an inadequacy of the conventional ap-

**8340 ** **H. M. LU A N D J. R. HARDY **

### 42

proach has been found during a study of phase transitions
in Rb2ZnC1,. lo- **l 2 ** Specifically, the short-range potential

for the z n z f -C1- ion pair computed from the electron charge densities of the free z n 2 + and C1- ions was mani- festly too hard, and an overall reduction of this potential had to be adopted to give good agreement with the exper- imental Zn-C1 bond length. Also some distortions of the z n ~ 1 2 - ion occurred, probably resulting from the combination of lack of intramolecular bond-angle stiffness and full ionicity. Moreover, the theoretical structures fail to give the correct orientations of the z n ~ l ? - , which clearly indicates defects in the descrip- tions of the intermolecular interactions. This inadequacy of the method would become even more obvious if it-were used to treat K2Se04, since the required closed-shell elec- tron charge-density distribution would give selenium the unrealistically large ionicity of 6 + .

In this work we present a major extension of the
Gordon-Kim approach to treat ionic molecular crystals,
as exemplified by K,Se04. The essence of this is to treat
the molecular ions as single entities and give separate
considerations to the intramolecular and intermolecular
interactions. The starting point of our new approach is
to perform *ab initio *quantum-chemistry calculations for
the whole molecular ions, i.e., ~ e 0 , * - . From these calcu-
lations one obtains an energy expression for the molecu-
lar ion to evaluate the intramolecular interactions, and
one also obtains the electron charge distribution for the
calculation of the intermolecular interactions. As will be
shown, this approach produces very accurate potential-
energy surfaces for K2Se04.

On the basis of the resultant *ab initio potential-energy *
surface we first performed symmetry restricted static re-
laxations for the room-temperature Pnam and the lower-
temperature P n ~ 2 ~ structures of K,SeO,. Apart from an
overall shorting of the lattice constants, which is a rather
general feature for large unit-cell simulations using
Gordon-Kim potentials, the theoretical structures agreed
very well with the experimental data, indicating that our
potentials are very satisfactory.

The method of molecular dynamics was then used to
simulate directly the dynamical states of K2Se04 at
different temperatures. By quenching a supercell of 336
ions, we studied the transition of K2Se04 from its room-
temperature *Pnam * structure to its lower-temperature
*Pna2, *structure. However, since this simulation uses
periodic boundary conditions, it cannot directly simulate
the incommensurate structure of K,Se04. Nonetheless,
since both the incommensurate and the subsequent fer-
roelectric lock-in transitions originate from the same
basic structural instability, they appear as a combined
transition in the simulation. By computing a convenient-
ly defined order parameter for the simulated structures at
different temperatures, we can infer temperatures for the
onset and the lock-in of this transition. These tempera-
tures match closely the experimental values to within the
statistical uncertainties of the supercell molecular-
dynamics simulations associated with finite sample size.

To investigate the structural instability from a different point of view, we then calculated the dispersion curves for the Pnam structure of K,Se04 along the a* direction

using our ab initio potentials. It was found that the most unstable point indeed occurs near f a * , as is the case for experiment.

Based on this excellent agreement between static and

### -

dynamic simulations and the experimental data, we shall then discuss the origin of the structural instability re- sponsible for the phase transitions. It will be shown that a double-well type of structure in the potential-energy surface for the rotation of the ~ e 0 , ~ - ions is the driving mechanism of the transitions. A new and stable structure is found, which has a singlet rather than the triplet struc- ture found experimentally. Although this new structure has a potential energy slightly lower than the triplet*Pna2,*structure, it cannot be accessed by the supercell molecular-dynamics simulations. An explanation for this is given in terms of the difference between the entropies of the singlet and the triplet structures.

This paper is organized as follows: in Sec. I1 we
present the procedure for obtaining the intramolecular
and intermolecular potentials from quantum-chemistry
calculations. section111 gives the results of the static re-
laxations for both the room-temperature *Pnam *and the
lower-temperature *Pna2, *structures. In Sec. IV we de-
scribe molecular-dynamics calculations to simulate the
phase transitions in K2Se04. Section V considers qualita-
tively the lattice instability from the point of view of lat-
tice dynamics and discusses the driving mechanism of the
transition. Section VI concludes the paper. It should
also be noted that a Brief Report of the present work has
been published.'4

**11. CALCULATIONS OF THE AB INITIO **
**INTERMOLECULAR AND INTRAMOLECULAR **

**POTENTIALS **

As pointed out in the Introduction, our starting point
is to perform *ab initio *quantum-chemistry calculations
for the ~ e 0 2 - molecular ion. Our calculations were
made for an isolated ~ e 0 2 - ion and thus did not include
a background crystal field. This is justified by the finding
that, while the oxygen sites in K2Se04 are the only sites
with nonnegligible crystal electric fields, over 90% of the
contribution to these fields is from the other ions in the
same

### s~o,*-

group, rather than from the rest of the lat- tice. This is found to be true for both the room- temperatures*Pnam*and the lower-temperature

*Pna2,*structures.

### 42

*STUDIES OF THE PHASE TRANSITIONS IN K,SeO, 8341*

**Ab****initio**of the intramolecular interactions, i.e., the Se-0 and 0-0 interactions within the same Se0:- ion. Such a descrip- tion is adequate as far as studies of the phase transitions are concerned, since throughout, in the Pnam, incom- mensurate, and Pna2, phases, the ~ e 0 , ~ - ions stay as near perfect tetrahedra, in agreement with experiment.

These quantum-chemistry calculations were performed
using the **GAUSSIAN86 **program.15 For the oxygen atoms
the standard 6-31G basis set was used, and for Se atom,
the STO-3G basis was employed. For both atoms single
first polarization functions were added to the basis sets.

We now turn to intermolecular interactions, i.e., those between the ion pairs, K-Se, K - 0 , and Se-Se and the pairs Se-0 and 0 - 0 , where the ions in a pair belong the different molecular groups. For these ion pairs there is no electron covalency involved, therefore the Gordon- Kim electron-gas model should still be appropriate for the calculation of these potentials. To perform these cal- culations we need the electron charge distributions of the individual K, Se, and 0 ions. For K we simply use the closed-shell charge distribution for free K ion,16 while for Se and 0 we extract their charge densities from the charge density of the whole ~ e 0 ~ ~ - ion obtained in the self-consistent Hartree-Fock calculation for the opti- mized structure of ~ e 0 , ~ - . Briefly, this extraction is made in the spirit of Mulliken population analysis.'' The total electron charge density for the whole ~ e 0 ~ ~ - ion can be expressed as

where (dpi,p,it ) are the elements of the symmetric density matrix and

### xpi

is the ith contracted real Gaussian atomic orbital centered at atom*The terms with*

**p.***origi- nate from overlap of atomic orbitals centered at different atoms. In the Mulliken population analysis, the contri- bution to the total number of electrons from these terms, i.e., d,i,,,if(~,i IX,,~.), are equally distributed to the separate atoms. Accordingly, in the present case, we separate the contributions to these terms by adding d,i,,,i# (,yNi*

**p f p '**### lxpli,

) to the diagonal element dpi,,i (and d,.i,,ei (*x~,;, *

### lxpi

) to d,,,i.,,.i. ). Then we have a density matrix d,i,,pi, block diagonalized with respect to different atoms, in terms of which the total charge density can be written approximately asConsequently we write * p( *r = &p,(

**r),**with p,(r) =

### z.

I,l .,dl ~ l , p r ~ ~ p i ~ ~ i ~ , . . defining the charge-density distribu- tion of atom*If we integrate the charge density p,(r) for each atom, the number of electrons obtained is exact- ly the same as given by Mulliken population analysis. The resultant ionicities for Se and 0 are 1.1504 and -0.7876, respectively, very different from the + 6 and -2 values for the closed-shell configurations of these atoms.*

**p.**We should like to emphasize that such a separation of the total charge density of the selenate ion into com- ponents for its constituent atoms is meaningful only for

the calculation of the intermolecular potentials. It is used to provide an approximate but effective representa- tion of the interactions external to the selenate group and is not to be understood as an intramolecular assignment of electrons to the individual atoms, since these electrons are intrinsically shared by all the atoms in the group, through the Hartree-Fock calculations.

We note that, in principle, the total charge distribution of the Se0:- ion produced by the quantum-chemistry calculations depends on the configuration of this ion, as do the charge densities of the individual atoms obtained by the procedure explained above. However, because of the bond and bond-angle stiffness, the Se0;- ions do not alter their shapes drastically in the different phases or in thermal motions, even at room temperature, as will be seen from our molecular-dynamics simulations at such temperatures. Therefore we assume the ions within ~ e 0 , ~ - to have rigid electron charge distributions and we take these distributions as those calculated for the opti- mized structure of Se0:-, since this structure is very close to the actual structure of the selenate ions in the crystal. We should again stress that this "rigid-ion" as- sumption only concerns calculations of the intermolecu- lar interactions. For the interactions within the ~ e 0 , ~ - group, which could be much more sensitive to the charge-density variations, this assumption may be in- valid. But our approach to the description of these in- teractions, described at the beginning of this section, au- tomatically includes the effect of such charge-density variations.

In the Gordon-Kim model and charge distributions of the two atoms are spherical.13 The charge distributions for the atoms obtained from the separation described above do not necessarily meet this requirement, due to the unequal populations on the different components of the p and/or d orbitals, and therefore have to be modified further. Our method is to condense the p and d orbitals and to replace them by spherical orbitals that contain just the radial parts of the p or d orbitals. For example, for a p orbital, we add together all the elements in the 3x3 block in the density matrix corresponding to the p,, p,, and p,, orbitals to form a diagonal element for a new spherical orbital that has just the radial part of the p or- bital. We also add the three elements that involve one of the three components and another different orbital to make an off-diagonal element between the new spherical orbital and that particular orbital. The resultant charge distribution consists of a condensed matrix with a num- ber of spherical orbitals, corresponding to each shell of the electronic configuration, and is therefore spherical.

**8342 **

**H. **

**M.**

**LU **

**AND J. R. HARDY**-

**42**

they are very small on the outskirts of the ~e0:- group. Since it is the overlap of these outskirts that contributes most to the Gordon-Kim potentials external to the ~e0:- ion, our approximate charge densities for the in- dividual atoms should be sufficiently accurate, since they are used only for the intermolecular interactions. The ex- cellent agreements between theory and experiment to be presented later will show that this is indeed the case. While the present procedure for extracting the spherical charge densities for individual atoms appears rather crude; it is, however, direct and simple, and allows sys- tematic improvement if necessary for other systems.

Finally, it should be noted that this method for extract- ing the spherical charge-density distributions for indivi- dual atoms is such that it will be exact for the charge dis- tribution of a closed shell, as can be easily shown. This may be important, especially for atoms that contain a large number of electrons, e.g., for Se. For these atoms most of the electrons are inner core electrons that retain a closed-shell structure.

Using the resultant spherical charge-density distribu- tions for Se and 0 , and the closed-shell charge-density distribution for free K', we then calculated the Gordon- Kim pair potentials between these ions. The long-range Coulomb interactions are determined from the fractional ionicities of the Se and 0 atoms, 1.1504 for Se and -0.7876 for 0, and the ionicity

### +

1 for K'. The short- range potentials were calculated numerically over a range of separations from 2 to 12 a.u. for all the ion pairs; for greater separations these potentials are less than lo-' hartree.These numerical short-range potentials were then fitted to the analytic form employed previously11

with r,=2 and r,=12 a.u., to avoid numerical
differentiation. It was found that polynomials of degree
N = 8 are enough to provide fits with errors of less than
0.1 % at every point. To complete the fit, a core function
u ( r ) = A + ~ / r ~ , r l r , , and a tail function U ( r )
=Cexp( --or2), r **1 **r,, were attached by requiring that
the votential and its first derivative be continuous at the
points of attachment.

An alternative to the present description of the inter- molecular interactions is to use, rather than ion-to-ion pairwise potentials, potentials derived for the molecular groups from their unmodified charge densities as has been done for ~ r - C O . " However, this requires that the

### s~o:-

ion be treated in the dynamics as a rigid rotor. The resultant complexities and ambiguities are such that this is clearly a worse approach: the single-atom pairwise potential is both more accurate dynamically and an unambiguous zero-order approximation that can be sys- tematically improved if necessary.**111. STATIC Pnam **

**AND Pna 2 ****STRUCTURES OF K2Se04 **

With the intramolecular and intermolecular potentials determined, we performed static relaxation calculations

for the room-temperature Pnam and low-temperature Pna2, structures of K,SeO,. These relaxations gave the crystal structures that are at extremes of the theoretical potential-energy surface-where the forces on the basis ions are zero. A comparison of the positions of the ions in these structures with the positions determined by ex- periment provides a sensitive test of the validity of the theoretical potential-energy surface.

First we consider the room-temperature Pnam struc- ture of K2Se0, (space group

**D::). **

Figure 1 shows the
projections of the experimental positions2 parallel to eath
of the tbree orthorhombjc axes (a=7.661 A,
b = 10.466 A, and c =6.003 A ). The prototypic pa-
rameters for the experimental structure2 are given in
Table I in parentheses.
**D::).**

Our relaxation started from the experimental structure and was subject to the constraints of Pnam symmetry, i.e., only the parameters in the parentheses in Table I and the lengths of the lattice constants a,b,c were allowed to vary. The minimization was for an infinite lattice, ob- tained by applying periodic boundary conditions, and fol- lowed a Newton-Raphson algorithm. The standard tech- nique of the Ewald sum was used for the calculation of the lattice energy and forces, etc.

The relaxed structures have zero forces on the basis
ions and zero forces of constraint. Projections of the ion
positions in the relaxed structure af;e shown in yig. 2.
The latticeo constants are a =7.261 A, b =9.859 A, and
c = 5.670 **A. ** The relaxed prototypic parameters are
given in Table I along with the experimental values in
parentheses.

As can be seen both from Fig. 2 and from the prototyp- ic parameters given in Table I, our relaxed structure agrees very well with experiment, as far as the reduced (fractional) basis vectors are concerned. The largest difference between theory and experiment is only 0.0168, for the y / b paramety of K(2), which corresponds to a change of 0.1759 A in the atomic position. This discrepancy is well below the thermal fluctuation of the atomic positions at room temperature.

* Ab initio *STUDIES OF THE PHASE TRANSITIONS IN K2Se0,

FIG. 1. Projections of the experimentally determined average structure of K2SeO4 in the *Pnam *phase. Unit vectors indicate the
directions of the lattice basis vectors. **A **unit vector pointing out of the figure is represented by a circle and the one pointing into the
figure is represented by a dot. Bonds (straight lines) connect each Se and the nearest four 0 ions.

significant, the near uniformly contracted theoretical
structure should still preserve those basic symmetries of
the system relevant to the phase transitions under study.
In particular, the ~ e 0 2 - ions will lie on the imperfect
sixfold helices that replace their exact counterparts in the
"ideal" hexagonal structure. In this situation there is n o
longer any reason to expect that a11 *exact *threefold repeat
will render the helical component of the free energy sta-
tionary, rather than contrary, hence an incommensurate
phase can develop. One can also argue this by consider-
ing the torques between adjacent molecular ions; if one
examines the situation closely, it becomes apparent that,
just as one has to impose vanishing surface stresses ex-
plicitly when periodic boundary conditions have been as-
sumed; so too does one have to relax the surface torques
in the emergent helices. When the helices are regular the
only nonzero torques, about the helical axis, are in the
surface cells and their relaxation only perturbs the sur-

face structure. However, when the helices are nonuni-
form and distorted *within a unit cell *there will exist a net
torque about the helical axis for each unit cell, which in
the infinite lattice, has to be offset by counter torques
from ions outside the helix. Clearly such a situation is
metastable with respect to any structural change that will
reduce these torques. This is provided at the surfaces.
Clearly the "unwinding" that relaxes the surface torques
for regular helices also permits a further unwinding to
reduce uniformally the torques *within *each unit cell.
This is a bulk effect and it appears as a finite uniform
change in the average pitch of the helices that n o longer
has to be commensurate with the lattice constant.

I n a previous study of Rb,ZnCl, (Ref. 10) it was found
that a static relaxation for the *Pnam * structure using
Gordon-Kim potentials computed from closed-shell
charge densities of ions with full ionicity gave a structure
that differs from the experimental structure in several as-

TABLE I. Prototypic atomic positions for K2Se04 in the relaxed *Pnam *structure. Experimental
values (Ref. 9) are given in parentheses.

**Wyckoff **

Prototype *x / a * **Y **/ b *z ***/C ** designation

Se 0.2324 (0.2242) 0.4203 (0.4200) - 4 I 4(c)

K(1) 0.1589 (0.1705) 0.0892 (0.0843) - 4 I 4(c)

K(2) 0.9869 (0.9943) 0.6927 (0.7095) - 4 **I ** 4(c)
O(1) 0.3074 (0.2931) 0.3432 (0.3471) 0.0183 (0.0271) 8(d)
O(2) 0.3 136 (0.3024) 0.5728 (0.5644) - 4 I 4(c)

**H. M. LU AND J. R. HARDY **

FIG. 2. Projections of the theoretical structure obtained by static relaxation with * Pnam *constraint.

pects: the Zn-C1 bond lengths were 10% too large, the significantly in the present structure, as is evident from ~n~1:- ions were distorted from near perfect tetrahedra Fig. 2 and Table I.

and rotated so that no Zn-C1 bond was parallel to the a Next we performed a static relaxation for the lower-
axis. These discrepancies also appeared for K2Se0, when temperature ferroelectric structure (space group *Pna2,) *
we used Gordon-Kim potentials computed from the of K,SeO, to examine further the potential-energy sur-
closed-shell charge distributions for se6+, 0 2 - , and K + face. Figure 2 shows projections of the experimental po-
ions. However, none of these discrepancies exists sitions parallel to each of the three orthorhombic axes

TABLE **11. **Prototypic atomic positions for K,SeO, relaxed within Pna2, constraints.

Wyckoff
Prototype **x ****/ a ***Y / b * z */ c * designation

*42 *

**Ab****initio**STUDIES OF THE PHASE TRANSITIONS IN K2Se0,

( a =22.716

**A, **

b = 10.339 **A, **

and c =5.967 **A). **

l 9 The
prototypic atomic positions for the experimental struc-
ture4 are given in Table **I1**in parentheses. Comparing the structure in Fig.

**3**with that of Fig. 1, we see that the unit cell in the Pna2, structure can be considered as formed by tripling the unit cell in the Pnam structure and then slightly modulating along the a direction the orientations of the ~ e 0 , ~ - groups and the positions of the K + ions.lg This tripling of the structure is a result of a lock-in from the incommensurate phase that exists between the Pnam and Pna2, phases.4,19

With the Pna2* symmetry constraints we performed a
static relaxation starting from the experimental structure
given in Fig. 3, and obtained the relaxed structure in Fig.
4 with the prototypic parameters given in Table **11. **The
lengths of t)e lattice axeso in the relaxed strusture are
a=21.752 **A, ** b=9.845 A, and c=5.715 A, again
shorter than the experimental values (4.2% for a, 4.8%
for b, and 4.2% for c) but no worse so than for the Pnam
phase.

As can be seen from comparing the structure in Fig. 4
with that in Fig. 3, our relaxation gives a close fit to the
experimental data. The largest discrepancy in the re-
duced basis positions is (cf. Table **11) **0.033 for the

### z

coor- dinate of 0(8), which would mean an actual displacementFIG. **3. **Projections of the experimentally determined average
structure of K,SeO, in the * Pna2, *phase. Note that the a axis is
approximately triple that in the

*structure in Fig. 1.*

**Pnam**FIG. 4. Projections of the theoretical structure obtained by
static relaxation with * Pna2, *constraint.

of 0.2

**A **

if the experimental lattice constants are used.
This is wellounder the half width of the thermal fluctua-
tion (0.34 **A)**found by experiment.19 Overall the basic modulation in the experimental structure is closely repro- duced, although the amplitude of the modulation is slightly larger, as is to be expected from a comparison of the static modulation with the experimental dynamical average.

The theoretical P n ~ 2 ~ structure of K2Se04 in Fig. 4 possesses a spontaneous polarization along the c direc- tion as found by experimentU2O Its magnitude is only 0.023 p ~ / c m 2 , smaller than the experimental value of 0.07 p Y c m 2 at 80 K. Again such a direct comparison of the static and average values must be made with caution, since the size and sense of the electronic contribution to the spontaneous polarization could be important.

IV. DYNAMICS SIMULATIONS OF THE PHASE TRANSITION

**8346 ** **H. M. LU AND J. R. HARDY ** - **42 **

governs the phase transition.

The sample for our simulation consisted of twelve of
the *Pnam *unit cells of K2Se0,, in total *336 *ions. This su-

percell was obtained by first tripling the unit cell in the **a **

direction to obtain a cell that is consistent with the unit

cell of the *Pna2, *ferroelectric structure. Such tripling is

obviously necessary to allow the phase transition to

occur. Then the tripled cell was doubled both in b and **c **

directions to lessen artificial correlations in those two directions. Our simulations follow a constant- (zero-) pressure algorithm2' and are made for infinite samples by employing periodic boundary conditions. T o make the simulations-as realistic as possible, no restriction was ap- plied (besides the periodic boundary condition) to the su- percell, i.e., all of the ion positions and all of the lattice vectors were allowed to change during the simulations. The time increment between two successive steps in the

simulations was *0.005 * ps, which was found to be

sufficiently short.

Starting from the experimental *Pnam *structure, the

sample was first sufficiently relaxed to be as free of experi- mental information as possible, while it was maintained

at T = *300 *K . We then performed a molecular-dynamics

"quench" by gradually reducing the total kinetic energy of the sample in stages to zero. At each step the sample

was allowed to equilibrate for *2 *ps and the average tem-

perature and average positions of the ions for this tem-
perature were calculated. We found that we could indeed
reproduce realistically the experimentally observed
*Pnam -Pna *2, phase transition.

Figures *5 *and 6 shows the structures at *T = 3 0 0 * and

*57 *K , respectively, both averaged over 2 ps. I n these

figures, the average Se-0 bonds are indicated by straight lines and the thermal motions of the ions are given by el- lipsoids centered at the average positions.

Clearly the structure in Fig. 5 is virtually the same as

the experimental *Pnam *structure. The supercell is orthp-

rhombic wit) the average lattite constants *a *= 2 *1.9 17 *A,

*b = 19.859 *A, and c = *11.488 ***A. **In particular, the aver-
aged structure clearly maintains the threefold repeat

along a and twofold repeat along b and * c , *within the pre-

cision of the simulation. If the supercell is divided to 12

cells, each of them fits very closely the experimental
*Pnam *structure in Fig. *1, *with the lattice axes, as expect-

ed, shorter than the experimental values by *4.6% * for *a , *

*4.9% * for *b, *and *4.3% * for c. (Note these fits are slightly
better than those obtained in Sec. I11 from static relaxa-
tion.)

The large (about *k 0 . 5 *a.u.) amplitudes of the thermal

motions of some of the oxygen ions, as seen in Fig. 5, in- dicate that the crystal at this temperature is actually in a dynamical disordered state. The shapes of thermal ellip- soids show that this disorder is associated with the rota- tions of the selenate groups. In a previous Raman mea-

surement of the internal mode f r e s ~ e n c i e s , ~ ' more lines

were found than predicted by the conventional factor

group analysis for the perfect *Pnam *symmetry. **A **hy-

pothesis was then made that the selenate ions were orien- tationally disordered; this is now clearly confirmed by our present simulation.

When the temperature was lowered to 57 K , the sys-

tem transformed to the structure shown in Fig. 6. Com-

paring it with the room temperature structure in Fig. 5,

we see that while double periodicity along b and * c *direc-

tions was preserved, modulation occurred along the **a **

direction, resulting in the loss of the original threefold periodicity. Evidently the resultant tripled structure

closely fits the *Pna2, *structure of K2Se0,. The basic

modulation again agrees well with that in Fig. *3, *al-

though the amplitudes are again slightly larger. In fact,

when further cooled to T *=O * K , this structure agrees

closely with the theoretical *Pna 2 , *structure in Fig. *4 *both

in ionic positions and potential energy.

Having shown that our molecular-dynamics (MD)

simulations can indeed reproduce the transition of

K,SeO, from its *Pnam *phase to the *Pna2, *phase, we now

**42 **

- * Ab *initio STUDIES OF THE PHASE TRANSITIONS IN K2Se04

**8347**

seek to monitor the transition more precisely. Ideally, following the order parameter of a transition as a func- tion of temperature is the best way to locate the transi- tion temperature. However, it was shown experimental- ly4 that the primary order parameter is the amplitude of the lattice distortion that is characterized by a wave vec-

tor * q = f ( *1

**-6)a***in the

*phase, with*

**Pnam***being the*

**a***first reciprocal-lattice vector along the [loo] direction.
Even if S=O, this order parameter would be difficult to
calculate for a supercell that contains many * Pnam *cells
and a large number of ions, and therefore cannot be used.
However, since the modulation that induces the phase
transition involves the rotations of the ~e0:- ions (cf.
Figs. 5 and 61, the deviations of the Se-0 bonds from
their orientations in the

*structure can be employed*

**Pnam**FIG. 6. Structure of K,Se04 at * T=57 *K obtained from the
supercell molecular-dynamics "quenching."

*0 * 100 *2 0 0 * *3 0 0 *

T E M P E R A T U R E ( K )

FIG. **7. **Theoretical ( **X ) **and experimental (

*o order parame- *

ter values as function of temperature.

to monitor the phase transition. Thus we calculated the
rms values of this deviation by comparing the average
structures at different temperatures with the static * Pnam *
structure and employed that as an order parameter. To
obtain better statistics, we again increased our supercell
size to

**3a**X

*X*

**2b****4c**(672 ions), and extended the averaging time from 2 to 40 ps. The resultant order parameter R is plotted in Fig.

**7**as a function of temperature, along with the value of R for the experimental

*structure at 80 K."*

**P n ~ 2 ~**Despite the unavoidable noise, even at room tempera- ture, Fig. 7 clearly shows that the onset of the transition lies in the range 120- 140 K, which corresponds closely to that of the incommensurate phase transition,

*( T , *= 129.5 K), and the transition is virtually complete at

about the lock-in ferroelectric transition temperature
*Tc=93 *K, where our order parameter is in close agree-
ment with the experimental value. The behavior of R at
about 200 K was observed in several simulations; it is
probably a dynamical

### ,

but slow, precursor to the main transition. To clarify this point completely would require an even longer computation for a still larger number of ions, and this is beyond our computing resources and would in any case, not be warranted by the minor significance of this point.**V. DISCUSSION **

The excellent agreement between theory and experi-
ment described in Secs. I11 and IV leads us to conclude
that we have indeed found a very realistic * ab initio *
potential-energy surface for K2Se04. We shall now dis-
cuss how this potential-energy surface provides a first-
principles explanation of the driving mechanism of the
phase transitions in K,Se04.

**8348 ** **H. M. LU AND J. R. HARDY ** - **42 **

curves were measured for K,SeO, in its * Pnam *phase near
and above

**Ti. **

It was found that the lowest-lying **Ti.**

**2, **

**2,**

transverse optic branch propagating along the [I001
direction softens as temperature is lowered. The
minimum in this branch was at q=0.31a* and ap-
proached zero at the incommensurate transition tempera-
ture *T i , *thus revealing the soft-transverse-optic mode re-
sponsible for driving the phase transition. This mecha-
nism was studied by lattice-dynamical calculations within
the quasiharmonic approximation5 using potentials deter-
mined from the static equilibrium constraints and the ex-
perimental zone-center frequencies. This study success-
fully reproduced the softening of the 8, optical phonon
with the lowest soft mode in the vicinity of q = a 8 / 3 .
Thus it is of interest to see what dispersion curves are
produced by our present *ab initio *potentials. Although
our calculation was made for the static structure and
therefore cannot be directly compared with the experi-
mental data,4 it does, however, reveal the nature of the
potential surfaces and possible competing instabilities.

This lattice-dynamics calculation was performed for
the [loo] (8) direction and the lowest eight branches of
the dispersions are shown in Fig. 8 (the higher branches
are basically irrelevant to the discussion). This figure
displays the angular frequency squared ( * w 2 ) *divided by

**w**versus wave vector q; negative values therefore represent

FIG. 8. Dispersion curves for the theoretical * Pnam *structure
in Fig.

**2.**

imaginary frequencies.

The appearance of several negative branches in Fig. 8
indicates that the theoretical *Pnam *structure is actually
unstable. This seems surprising since the *Pnam *structure
was reached by our static relaxation, and all the forces on
the ions and the stresses were zero for this structure. The
probable explanation is that the *Pnam *structure is not at
an absolute minimum but is at a fairly broad saddle point
on the potential-energy surface.

The lowest branch in Fig. 8 has X2 symmetry and does
meet a * 2 , *branch at the zone boundary. This at least
matches partially with experiment,4 although the

*branch here is not an acoustic phonon and is also nega- tive over the whole range. As pointed out previously, the present calculation does not include the temperature effects, and it is misleading to compare the present results either with experiment4 or with the previous theoretical study,5 where temperature effects were included by the quasiharmonic approximation. However, Fig. 8 does show that the absolute minimum, representing the dom- inant instability, occurs at q=0.304a*, very close to the experimental soft phonon wave vector q=O. 31a*. Thus as far as the symmetry of the instability is concerned, our calculation agrees well with experiment. This result is complementary to our earlier supercell MD simulation of the cell-tripling transition, in the sense that it demon- strates, in some measure, that the tripling is not a mere consequence of the choice of the supercell.*

**2 ,**To see if the *Pnam *structure has similar instabilities
along other directions, we calculated the dispersion
curves along both the b and * c *directions. We found that
the lowest unstable points are at the zone center. Since
this is obviously a direct consequence of the negative
values at the zone center in Fig. 8, there are apparently
no new instabilities. We also calculated the dispersion re-
lations for the

*Pna2,*structure and found no imaginary branches. This is to be expected since this structure is stable down to zero temperature against molecular- dynamics relaxations.

The lowest 2, branch in the dispersion shown in Fig. 8
has negative values over the whole range, indicating mul-
tiple instabilities in the system, rather than at a single un-
stable point near q = t a * , as found by experiment. The
most interesting of these is at the zone center, involving
motions of the ions without changing the periodicity of
the lattice. Since the normal coordinate analysis shows
that the * 8, *branch involves essentially rotations of the
selenate groups, it is instructive to study the zone-center
instability to characterize these rotations which are, after
all, the basic origin of the instability in the system.

We thus performed molecular-dynamics relaxation for
a single cell of K2Se04, without any constraints besides
the periodic boundary condition, which only permits the
zone-center instabilities. When we cooled the sample to
T = O K , a new stable structure, distinct from the *Pnam *

### 42

**Ab****initio****STUDIES OF THE PHASE TRANSITIONS IN K2Se04**

**8349**

mirror image of the other structure. I n Fig. 9 we show the projections of ions along the a directions in these two structures. If we compare Fig. 9 with Fig. l(a), the pro- jection of ions along the a direction in the Pnam struc- ture, we see that the two new structures in Fig. 9 are formed by rotations of the selenate ions and shifts of the potassium ions from the Pnam positions. While the shift amplitudes are equal in both, the signs of the displace- ments are opposed. The potential energies of both these structures are exactly equal at 12.3 meV per formula unit below that of the theoretical Pnam structure.

Thus we conclude that for a single *Pnam * cell the
potential-energy surface has a double-well shape with the
*Pnam *structure at the top and the new structures in Fig.
9, respectively, at the bottoms of the two wells. When
the periodicity along the a direction is changed, this dou-
ble well generates a multiple-well structure on the total
potential-energy surface, which is the origin of the
*Pnam-Pna2,, *cell-tripling transition. (We also checked
by MD that the single-cell double-well structure was not
affected by periodicity changes along the b and c direc-
tions.)

T o illustrate better this double-well potential-energy
surface, we then calculated the lattice potential energies
as we "stepped" from the *Pnam *structure to one of the
two new structures in Fig. 9, say [Fig. 9(a)], by changing
each coordinate by *2.5% *during each step. In Fig. 10 we
show these energies as a function of the fractional
changes in coordinate d. When we performed the similar
calculations for stepping from the Pnam structure to the

FIG. 10. Lattice potential energy (meV per formula unit) as a
function of the fractional displacement from the *Pnam *structure
* ( d *=O%) to the singlet structure in Fig. 9(a) ( d = 100%).

other new structure [Fig. 9(b)], i.e., using negative values for fractional changes d, we obtained identical results to those in Fig. 10. This conclusively demonstrates that we indeed have a double-well type of energy surface.

We then performed similar calculations of the potential
energy as we "stepped" from the Pnam structure to the
*Pna2, *structure, and show these energies in Fig. 11.
Since the Pna2, structure can be formed from the Pnam
structure in three different ways corresponding to the
three equivalent ways of defining the unit cell in the
*Pna2, structure, the potential surface of Fig. 11 is triply *
degenerate. While Figs. 10 and 11 display the basic
features of the potential-energy surfaces, they should not
be taken too literally, since the linear and equal stepping
between the structures may not be the best path for the
real system. For example, the very shallow dips around
d = O in Fig. 11 could be misleading and should therefore
be ignored. It can be seen, by comparing Fig. 10 with
Fig. 11, that the new singlet structures in Fig. 9 have a
minimum potential energy, lower than the *Pna2, *struc-

FIG. 9. **bc **cross sections of the two energetically equivalent
singlet structures of K,Se04 obtained from single-cell
molecular-dynamics relaxations. The lattice axes are given in
atomic units.

FIG. 11. Lattice potential energy (meV per formula unit) as a
function of the fractional displacement from the *Pnam *structure

8350 H. M. LU AND J. R. HARDY - 42

ture by about 1.6 meV per formula unit. However, our supercell molecular-dynamics "quenching" did not find either of these singlet structures, but rather selected the tripled P n a 2 , structure. This is not surprising if we more closely examine the quenching process. When the tem- perature is above

### -

130 K , the small (1.6-meV) difference in static energy between the two structures is negligible: thus the singlet and the triplet structure are effectively degenerate. Consequently as*kT*becomes less than

### -

10-15 meV, and the Pnam structure begins to trans- form, the state selected will be that of higher

**entropy.**Clearly, this is the P n ~ 2 ~ phase in which, for example,
the ~ e 0 ~ ' - ions have three rather than one possible
orientations. Subsequently, for the P n a 2 , structure to
transform to the rotated selenate single-cell phase, it re-
quires that at least one of the tetrahedra switch through
the P n a m configuration and as the system is cooled below
*k T - *10 meV, this becomes increasingly difficult. When
*kT *

### -

1 -2 meV (when the single phase would become pre- ferred energetically), the transformation is frustrated by the### -

10-meV activation barrier and the P n a 2 , phase persists.VI. CONCLUSION

In summary, we have developed a new approach to first-principles simulations specifically for ionic molecular

solids, and using this approach we studied the phase tran- sitions in K,Se04. By starting from a b initio quantum- chemistry calculations for the whole molecular ion we obtained an electron charge-density distribution that in- cludes self-consistently possible electron covalency within the molecular ion. From these distributions, a b initio in- terionic potentials were obtained by Taylor expansion of the energy for the intramolecular interactions, and by the Gordon-Kim electron-gas model for the intermolecular interactions. Using these potentials we successfully simu- lated both the Pnam and the P n a 2 , structures, and the phase transition between them, obtaining a transition temperature in good agreement with experiment. We also performed first-principles lattice-dynamics studies of K2SeO4 that revealed that the most instable point of the

Pnam structure is in the neighborhood of **q=+a*, **very
close to that observed experimentally. By investigating
the potential-energy surfaces pertinent to the phase tran-
sition, we found that a rotational double-well type of
motion is the basic origin of the instability in the system.

**ACKNOWLEDGMENTS **

This work was supported by the U.S. Army Research
Office (Research Triangle Park, **NC). **We should also like
to acknowledge many helpful discussions with Dr. P. **3. **

Edwardson and Dr. D. P. Billesbach.

'H. Z. Cummins, Phys. Rep. 185,211 (1990).

**2A. Kalman, J. S. Stephens, and **D. W. J. Cruickshank, Acta
Crystallogr. Sec. B 26, 145 1 (1970).

3N. Ohama, Mater. Res. Bull. 9, 283 (1974).

**4M. **Iizumi, J. D. Axe, G. Shirane, and K. Shimoaka, Phys. Rev.
B 15,4392 (1977).

5M. S. Haque and J. R. Hardy, Phys. Rev. B 21,245 (1980). 6L. L. Boyer, Phys. Rev. Lett. 42, 584 (1979). A fuller account

is given in Phys. Rev. B 23, 3673 (1981).

7L. L. Boyer, Phys. Rev. Lett. 45, 1858 (1980); 46, 1172 (1981). 8L. L.Boyer and J. R. Hardy, Phys. Rev. B 24, 2527 (1981). 9L. L. Boyer, J. Phys. C 17, 1825 (1984).

I0V. Katkanant, P. J. Edwardson, J. R. Hardy, and L. L. Boyer, Phys. Rev. Lett. 57, 2033 (1986).

"P. J. Edwardson, V. Katkanant, J. R. Hardy, and L. L. Boyer, Phys. Rev. B 35, 8479 (1987).

**I2V. **Katkanant, P. J. Edwardson, and J. R. Hardy, Phase Tran-

sitions 15, 103 (1989).

13R. G. Gordon and Y. S. Kim, J. Chem. Phys. 56,3122 (1971).
I4H. M. Lu and J. R. Hardy, Phys. Rev. Lett. 64, 661 (1990).
ISM. J. Frisch * et a!., *GAUSSIAN86 (Carnegie-Mellon Quantum

Chemistry Publishing Unit, Pittsburgh, PA, 1984).

I6E. Clementi and C. Roetti, At. Data Nucl. Data Tables 14, 177 (1974).

17R. S. Mulliken, J. Chem. Phys. 23, 1833 (1955).

I8G. A. Parker and R. T. Pack, J. Chem. Phys. 69, 3268 (1978). 19N. Yamada, Y. Ono, and T. Ikeda, J. Phys. Soc. Jpn. 53,2565

(1984).

20K. Aiki, K. Fukuda, H. Koga, and T. Kobayashi, J. Phys. Soc. Jpn. 28, 389 (1970).

21M. Parrinello and **A. **Rahman, Phys. Rev. Lett. 45, 1196
(1980).